LMucko/crystallography-open-database huggingface dataset:
Rietveld structure refinement of MgGeO3 post-perovskite phase to 1 Mbar Sample: A036, P = 105.4 GPa, T = 300 K
Kubo, A.; Kiefer, B.; Shim, S. H.; Shen, G.; Prakapenka, V. B.; Duffy, T. S.; American Mineralogist 93 (2008) 965–976; doi:10.2138/am.2008.2691

data_9010456
_publ_section_title
;
 Rietveld structure refinement of MgGeO3 post-perovskite phase to 1 Mbar
 Sample: A036, P = 105.4 GPa, T = 300 K
;
_journal_name_full               'American Mineralogist'
_journal_page_first              965
_journal_page_last               976
_journal_paper_doi               10.2138/am.2008.2691
_journal_volume                  93
_journal_year                    2008
_chemical_compound_source        Synthetic
_chemical_formula_structural     MgGeO3
_chemical_formula_sum            'Ge Mg O3'
_space_group_IT_number           63
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   2.5718
_cell_length_b                   8.3274
_cell_length_c                   6.3536
_cell_formula_units_Z            4
_cell_volume                     136.071
_database_code_amcsd             0004588
_diffrn_ambient_pressure         1.054e+08
_diffrn_ambient_temperature      300
_exptl_crystal_density_diffrn    7.074
_cod_original_formula_sum        'Mg Ge O3'
_cod_database_code               9010456
_amcsd_formula_title             MgGeO3
Rietveld structure refinement of MgGeO3 post-perovskite phase to 1 Mbar Sample: A038, P = 109.3 GPa, T = 300 K
Kubo, A.; Kiefer, B.; Shim, S. H.; Shen, G.; Prakapenka, V. B.; Duffy, T. S.; American Mineralogist 93 (2008) 965–976; doi:10.2138/am.2008.2691

data_9010457
_publ_section_title
;
 Rietveld structure refinement of MgGeO3 post-perovskite phase to 1 Mbar
 Sample: A038, P = 109.3 GPa, T = 300 K
;
_journal_name_full               'American Mineralogist'
_journal_page_first              965
_journal_page_last               976
_journal_paper_doi               10.2138/am.2008.2691
_journal_volume                  93
_journal_year                    2008
_chemical_compound_source        Synthetic
_chemical_formula_structural     MgGeO3
_chemical_formula_sum            'Ge Mg O3'
_space_group_IT_number           63
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   2.5677
_cell_length_b                   8.3132
_cell_length_c                   6.3453
_cell_formula_units_Z            4
_cell_volume                     135.446
_database_code_amcsd             0004589
_diffrn_ambient_pressure         1.093e+08
_diffrn_ambient_temperature      300
_exptl_crystal_density_diffrn    7.106
_cod_original_formula_sum        'Mg Ge O3'
_cod_database_code               9010457
_amcsd_formula_title             MgGeO3
Rietveld structure refinement of MgGeO3 post-perovskite phase to 1 Mbar Sample: A042, P = 100.2 GPa, T = 300 K
Kubo, A.; Kiefer, B.; Shim, S. H.; Shen, G.; Prakapenka, V. B.; Duffy, T. S.; American Mineralogist 93 (2008) 965–976; doi:10.2138/am.2008.2691

data_9010458
_publ_section_title
;
 Rietveld structure refinement of MgGeO3 post-perovskite phase to 1 Mbar
 Sample: A042, P = 100.2 GPa, T = 300 K
;
_journal_name_full               'American Mineralogist'
_journal_page_first              965
_journal_page_last               976
_journal_paper_doi               10.2138/am.2008.2691
_journal_volume                  93
_journal_year                    2008
_chemical_compound_source        Synthetic
_chemical_formula_structural     MgGeO3
_chemical_formula_sum            'Ge Mg O3'
_space_group_IT_number           63
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   2.5811
_cell_length_b                   8.3628
_cell_length_c                   6.3730
_cell_formula_units_Z            4
_cell_volume                     137.563
_database_code_amcsd             0004590
_diffrn_ambient_pressure         1.002e+08
_diffrn_ambient_temperature      300
_exptl_crystal_density_diffrn    6.997
_cod_original_formula_sum        'Mg Ge O3'
_cod_database_code               9010458
_amcsd_formula_title             MgGeO3
Rietveld structure refinement of MgGeO3 post-perovskite phase to 1 Mbar Sample: B017, P = 92.1 GPa, T = 1740 K
Kubo, A.; Kiefer, B.; Shim, S. H.; Shen, G.; Prakapenka, V. B.; Duffy, T. S.; American Mineralogist 93 (2008) 965–976; doi:10.2138/am.2008.2691

data_9010459
_publ_section_title
;
 Rietveld structure refinement of MgGeO3 post-perovskite phase to 1 Mbar
 Sample: B017, P = 92.1 GPa, T = 1740 K
;
_journal_name_full               'American Mineralogist'
_journal_page_first              965
_journal_page_last               976
_journal_paper_doi               10.2138/am.2008.2691
_journal_volume                  93
_journal_year                    2008
_chemical_compound_source        Synthetic
_chemical_formula_structural     MgGeO3
_chemical_formula_sum            'Ge Mg O3'
_space_group_IT_number           63
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   2.6001
_cell_length_b                   8.4123
_cell_length_c                   6.4099
_cell_formula_units_Z            4
_cell_volume                     140.203
_database_code_amcsd             0004591
_diffrn_ambient_pressure         9.21e+07
_diffrn_ambient_temperature      1740
_exptl_crystal_density_diffrn    6.865
_cod_original_formula_sum        'Mg Ge O3'
_cod_database_code               9010459
_amcsd_formula_title             MgGeO3
Rietveld structure refinement of MgGeO3 post-perovskite phase to 1 Mbar Sample: B018, P = 93.6 GPa, T = 1420 K
Kubo, A.; Kiefer, B.; Shim, S. H.; Shen, G.; Prakapenka, V. B.; Duffy, T. S.; American Mineralogist 93 (2008) 965–976; doi:10.2138/am.2008.2691

data_9010460
_publ_section_title
;
 Rietveld structure refinement of MgGeO3 post-perovskite phase to 1 Mbar
 Sample: B018, P = 93.6 GPa, T = 1420 K
;
_journal_name_full               'American Mineralogist'
_journal_page_first              965
_journal_page_last               976
_journal_paper_doi               10.2138/am.2008.2691
_journal_volume                  93
_journal_year                    2008
_chemical_compound_source        Synthetic
_chemical_formula_structural     MgGeO3
_chemical_formula_sum            'Ge Mg O3'
_space_group_IT_number           63
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   2.5987
_cell_length_b                   8.4107
_cell_length_c                   6.4079
_cell_formula_units_Z            4
_cell_volume                     140.057
_database_code_amcsd             0004592
_diffrn_ambient_pressure         9.36e+07
_diffrn_ambient_temperature      1420
_exptl_crystal_density_diffrn    6.872
_cod_original_formula_sum        'Mg Ge O3'
_cod_database_code               9010460
_amcsd_formula_title             MgGeO3
Rietveld structure refinement of MgGeO3 post-perovskite phase to 1 Mbar Sample: B019, P = 87.8 GPa, T = 300 K
Kubo, A.; Kiefer, B.; Shim, S. H.; Shen, G.; Prakapenka, V. B.; Duffy, T. S.; American Mineralogist 93 (2008) 965–976; doi:10.2138/am.2008.2691

data_9010461
_publ_section_title
;
 Rietveld structure refinement of MgGeO3 post-perovskite phase to 1 Mbar
 Sample: B019, P = 87.8 GPa, T = 300 K
;
_journal_name_full               'American Mineralogist'
_journal_page_first              965
_journal_page_last               976
_journal_paper_doi               10.2138/am.2008.2691
_journal_volume                  93
_journal_year                    2008
_chemical_compound_source        Synthetic
_chemical_formula_structural     MgGeO3
_chemical_formula_sum            'Ge Mg O3'
_space_group_IT_number           63
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   2.5971
_cell_length_b                   8.4089
_cell_length_c                   6.4064
_cell_formula_units_Z            4
_cell_volume                     139.908
_database_code_amcsd             0004593
_diffrn_ambient_pressure         8.78e+07
_diffrn_ambient_temperature      300
_exptl_crystal_density_diffrn    6.880
_cod_original_formula_sum        'Mg Ge O3'
_cod_database_code               9010461
_amcsd_formula_title             MgGeO3
Rietveld structure refinement of MgGeO3 post-perovskite phase to 1 Mbar Sample: B020, P = 89.5 GPa, T = 300 K
Kubo, A.; Kiefer, B.; Shim, S. H.; Shen, G.; Prakapenka, V. B.; Duffy, T. S.; American Mineralogist 93 (2008) 965–976; doi:10.2138/am.2008.2691

data_9010462
_publ_section_title
;
 Rietveld structure refinement of MgGeO3 post-perovskite phase to 1 Mbar
 Sample: B020, P = 89.5 GPa, T = 300 K
;
_journal_name_full               'American Mineralogist'
_journal_page_first              965
_journal_page_last               976
_journal_paper_doi               10.2138/am.2008.2691
_journal_volume                  93
_journal_year                    2008
_chemical_compound_source        Synthetic
_chemical_formula_structural     MgGeO3
_chemical_formula_sum            'Ge Mg O3'
_space_group_IT_number           63
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   2.5949
_cell_length_b                   8.4009
_cell_length_c                   6.4013
_cell_formula_units_Z            4
_cell_volume                     139.545
_database_code_amcsd             0004594
_diffrn_ambient_pressure         8.95e+07
_diffrn_ambient_temperature      300
_exptl_crystal_density_diffrn    6.898
_cod_original_formula_sum        'Mg Ge O3'
_cod_database_code               9010462
_amcsd_formula_title             MgGeO3
Rietveld structure refinement of MgGeO3 post-perovskite phase to 1 Mbar Sample: B038, P = 85.0 GPa, T = 300 K
Kubo, A.; Kiefer, B.; Shim, S. H.; Shen, G.; Prakapenka, V. B.; Duffy, T. S.; American Mineralogist 93 (2008) 965–976; doi:10.2138/am.2008.2691

data_9010463
_publ_section_title
;
 Rietveld structure refinement of MgGeO3 post-perovskite phase to 1 Mbar
 Sample: B038, P = 85.0 GPa, T = 300 K
;
_journal_name_full               'American Mineralogist'
_journal_page_first              965
_journal_page_last               976
_journal_paper_doi               10.2138/am.2008.2691
_journal_volume                  93
_journal_year                    2008
_chemical_compound_source        Synthetic
_chemical_formula_structural     MgGeO3
_chemical_formula_sum            'Ge Mg O3'
_space_group_IT_number           63
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   2.6018
_cell_length_b                   8.4259
_cell_length_c                   6.4161
_cell_formula_units_Z            4
_cell_volume                     140.657
_database_code_amcsd             0004595
_diffrn_ambient_pressure         8.5e+07
_diffrn_ambient_temperature      300
_exptl_crystal_density_diffrn    6.843
_cod_original_formula_sum        'Mg Ge O3'
_cod_database_code               9010463
_amcsd_formula_title             MgGeO3
Rietveld structure refinement of MgGeO3 post-perovskite phase to 1 Mbar Sample: B040, P = 79.2 GPa, T = 300 K
Kubo, A.; Kiefer, B.; Shim, S. H.; Shen, G.; Prakapenka, V. B.; Duffy, T. S.; American Mineralogist 93 (2008) 965–976; doi:10.2138/am.2008.2691

data_9010464
_publ_section_title
;
 Rietveld structure refinement of MgGeO3 post-perovskite phase to 1 Mbar
 Sample: B040, P = 79.2 GPa, T = 300 K
;
_journal_name_full               'American Mineralogist'
_journal_page_first              965
_journal_page_last               976
_journal_paper_doi               10.2138/am.2008.2691
_journal_volume                  93
_journal_year                    2008
_chemical_compound_source        Synthetic
_chemical_formula_structural     MgGeO3
_chemical_formula_sum            'Ge Mg O3'
_space_group_IT_number           63
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   2.6113
_cell_length_b                   8.4602
_cell_length_c                   6.4381
_cell_formula_units_Z            4
_cell_volume                     142.231
_database_code_amcsd             0004596
_diffrn_ambient_pressure         7.92e+07
_diffrn_ambient_temperature      300
_exptl_crystal_density_diffrn    6.767
_cod_original_formula_sum        'Mg Ge O3'
_cod_database_code               9010464
_amcsd_formula_title             MgGeO3
Rietveld structure refinement of MgGeO3 post-perovskite phase to 1 Mbar Sample: B041, P = 78.2 GPa, T = 300 K
Kubo, A.; Kiefer, B.; Shim, S. H.; Shen, G.; Prakapenka, V. B.; Duffy, T. S.; American Mineralogist 93 (2008) 965–976; doi:10.2138/am.2008.2691

data_9010465
_publ_section_title
;
 Rietveld structure refinement of MgGeO3 post-perovskite phase to 1 Mbar
 Sample: B041, P = 78.2 GPa, T = 300 K
;
_journal_name_full               'American Mineralogist'
_journal_page_first              965
_journal_page_last               976
_journal_paper_doi               10.2138/am.2008.2691
_journal_volume                  93
_journal_year                    2008
_chemical_compound_source        Synthetic
_chemical_formula_structural     MgGeO3
_chemical_formula_sum            'Ge Mg O3'
_space_group_IT_number           63
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   2.6127
_cell_length_b                   8.4674
_cell_length_c                   6.4413
_cell_formula_units_Z            4
_cell_volume                     142.499
_database_code_amcsd             0004597
_diffrn_ambient_pressure         7.82e+07
_diffrn_ambient_temperature      300
_exptl_crystal_density_diffrn    6.755
_cod_original_formula_sum        'Mg Ge O3'
_cod_database_code               9010465
_amcsd_formula_title             MgGeO3
Synthesis and crystal structure of the feldspathoid CsAlSiO4: An open-framework silicate and potential nuclear waste disposal phase
Gatta, G. D.; Rotiroti, N.; Zanazzi, P. F.; Rieder, M.; Drabek, M.; Weiss, Z.; Klaska, R.; American Mineralogist 93 (2008) 988–995; doi:10.2138/am.2008.2729

data_9010466
_publ_section_title
;
 Synthesis and crystal structure of the feldspathoid CsAlSiO4: An
 open-framework silicate and potential nuclear waste disposal phase
;
_journal_name_full               'American Mineralogist'
_journal_page_first              988
_journal_page_last               995
_journal_paper_doi               10.2138/am.2008.2729
_journal_volume                  93
_journal_year                    2008
_chemical_compound_source        Synthetic
_chemical_formula_structural     CsAlSiO4
_chemical_formula_sum            'Al Cs O4 Si'
_space_group_IT_number           33
_symmetry_space_group_name_Hall  'P -2n -2ac'
_symmetry_space_group_name_H-M   'P c 21 n'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   9.414
_cell_length_b                   5.435
_cell_length_c                   8.875
_cell_formula_units_Z            4
_cell_volume                     454.090
_database_code_amcsd             0004598
_exptl_crystal_density_diffrn    3.686
_cod_original_formula_sum        'Cs Si Al O4'
_cod_database_code               9010466
_amcsd_formula_title             CsAlSiO4
The crystal chemistry of Li in gadolinite
Camara, F.; Oberti, R.; Ottolini, L.; Ventura, G. D.; Bellatreccia, F.; American Mineralogist 93 (2008) 996–1004; doi:10.2138/am.2008.2748

data_9010467
_publ_section_title
;
 The crystal chemistry of Li in gadolinite
;
_journal_name_full               'American Mineralogist'
_journal_page_first              996
_journal_page_last               1004
_journal_paper_doi               10.2138/am.2008.2748
_journal_volume                  93
_journal_year                    2008
_chemical_compound_source        'Vico lake, Latium, Italy'
_chemical_formula_sum
;B0.8 Be1.08 Ca0.8 Ce0.24 Dy0.04 Er0.02 Eu2 Fe0.71 Gd0.04 La0.06 Li0.35 Mg0.02
 Mn0.03 Nd0.16 O10 Pr0.04 Si2 Sm0.04 Th0.14 U0.02 Y0.38 Yb0.02
;
_chemical_name_mineral           Gadolinite-(Y)
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 90.017
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   4.7708
_cell_length_b                   7.6229
_cell_length_c                   9.8975
_cell_volume                     359.946
_database_code_amcsd             0004599
_exptl_crystal_density_diffrn    7.216
_cod_original_formula_sum
;(Ca.8 Y.38 La.06 Ce.24 Pr.04 Nd.16 Sm.04 Eu2 Gd.04 Dy.04 Er.02 Yb.02 Th.14
 U.02) Fe.71 Li.35 Mn.03 Mg.02 Si2 Be1.08 B.8 O10
;
_cod_database_code               9010467
The effect of the hedenbergitic substitution on the compressibility of jadeite Sample: Jd0Hd100 at P = 0 GPa
Nestola, F.; Ballaran, T. B.; Liebske, C.; Thompson, R.; Downs, R. T.; American Mineralogist 93 (2008) 1005–1013; doi:10.2138/am.2008.2773

data_9010468
_publ_section_title
;
 The effect of the hedenbergitic substitution on the compressibility
 of jadeite
 Sample: Jd0Hd100 at P = 0 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1005
_journal_page_last               1013
_journal_paper_doi               10.2138/am.2008.2773
_journal_volume                  93
_journal_year                    2008
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Ca Fe O6 Si2'
_chemical_name_mineral           Jadeite
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 104.862
_cell_angle_gamma                90
_cell_length_a                   9.8447
_cell_length_b                   9.0234
_cell_length_c                   5.2509
_cell_formula_units_Z            4
_cell_volume                     450.847
_database_code_amcsd             0004600
_diffrn_ambient_pressure         0
_exptl_crystal_density_diffrn    3.655
_cod_original_formula_sum        'Ca Fe Si2 O6'
_cod_database_code               9010468
The effect of the hedenbergitic substitution on the compressibility of jadeite Sample: Jd0Hd100 at P = 3.80 GPa
Nestola, F.; Ballaran, T. B.; Liebske, C.; Thompson, R.; Downs, R. T.; American Mineralogist 93 (2008) 1005–1013; doi:10.2138/am.2008.2773

data_9010469
_publ_section_title
;
 The effect of the hedenbergitic substitution on the compressibility
 of jadeite
 Sample: Jd0Hd100 at P = 3.80 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1005
_journal_page_last               1013
_journal_paper_doi               10.2138/am.2008.2773
_journal_volume                  93
_journal_year                    2008
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Ca Fe O6 Si2'
_chemical_name_mineral           Jadeite
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 104.290
_cell_angle_gamma                90
_cell_length_a                   9.7553
_cell_length_b                   8.8998
_cell_length_c                   5.1923
_cell_formula_units_Z            4
_cell_volume                     436.848
_database_code_amcsd             0004601
_diffrn_ambient_pressure         3.8e+06
_exptl_crystal_density_diffrn    3.772
_cod_original_formula_sum        'Ca Fe Si2 O6'
_cod_database_code               9010469
The effect of the hedenbergitic substitution on the compressibility of jadeite Sample: Jd100Hd0, P = 0 GPa
Nestola, F.; Ballaran, T. B.; Liebske, C.; Thompson, R.; Downs, R. T.; American Mineralogist 93 (2008) 1005–1013; doi:10.2138/am.2008.2773

data_9010470
_publ_section_title
;
 The effect of the hedenbergitic substitution on the compressibility
 of jadeite
 Sample: Jd100Hd0, P = 0 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1005
_journal_page_last               1013
_journal_paper_doi               10.2138/am.2008.2773
_journal_volume                  93
_journal_year                    2008
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Al Na O6 Si2'
_chemical_name_mineral           Jadeite
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 107.624
_cell_angle_gamma                90
_cell_length_a                   9.4278
_cell_length_b                   8.5651
_cell_length_c                   5.2262
_cell_formula_units_Z            4
_cell_volume                     402.208
_database_code_amcsd             0004602
_diffrn_ambient_pressure         0
_exptl_crystal_density_diffrn    3.338
_cod_original_formula_sum        'Na Al Si2 O6'
_cod_database_code               9010470
The effect of the hedenbergitic substitution on the compressibility of jadeite Sample: Jd100Hd0, P = 3.14 GPa
Nestola, F.; Ballaran, T. B.; Liebske, C.; Thompson, R.; Downs, R. T.; American Mineralogist 93 (2008) 1005–1013; doi:10.2138/am.2008.2773

data_9010471
_publ_section_title
;
 The effect of the hedenbergitic substitution on the compressibility
 of jadeite
 Sample: Jd100Hd0, P = 3.14 GPa
;
_journal_name_full               'American Mineralogist'
_journal_page_first              1005
_journal_page_last               1013
_journal_paper_doi               10.2138/am.2008.2773
_journal_volume                  93
_journal_year                    2008
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Al Na O6 Si2'
_chemical_name_mineral           Jadeite
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 107.345
_cell_angle_gamma                90
_cell_length_a                   9.3488
_cell_length_b                   8.5013
_cell_length_c                   5.1856
_cell_formula_units_Z            4
_cell_volume                     393.395
_database_code_amcsd             0004603
_diffrn_ambient_pressure         3.14e+06
_exptl_crystal_density_diffrn    3.413
_cod_original_formula_sum        'Na Al Si2 O6'
_cod_database_code               9010471